Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles


 Poppy Smith
 2 years ago
 Views:
Transcription
1 Click Here for Full Article JOURNAL OF GEOPHYSICAL RESEARCH, VOL. 112,, doi: /2006jb004575, 2007 Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles Amy P. Chen, 1 Ramon Egli, 1 and Bruce M. Moskowitz 1 Received 15 June 2006; revised 3 February 2007; accepted 15 February 2007; published 2 August [1] Firstorder reversal curve (FORC) diagrams are rapidly becoming a standard tool for characterizing magnetic particles because they simultaneously incorporate information regarding magnetostatic interaction and domain states. The simplest interpretation of FORC diagrams of singledomain (SD) particles is based on the Neel interpretation of Preisach theory, which predicts that the FORC function is the product of a coercivity and an interaction field distribution. Although the underlying assumptions of this interpretation are not correct, a strictly quantitative model of weakly interacting SD grains proves that the distributions of coercivities and interaction fields can be retrieved from a FORC diagram. To test this model, we present the possibility of a quantitative interpretation of FORC diagrams, and we present measurements of samples containing magnetosomes from cultures of magnetotactic bacteria and from a lake sediment. Two samples are investigated under the electron microscope to characterize the geometrical arrangement of the particles. We find that the clustering of otherwise similar particles has a strong influence on FORC diagrams. We also obtained a crude estimate of packing densities form the FORC diagrams, which were consistent with transmission electron microscopy observations and measurements of the anhysteretic remanent magnetization. Citation: Chen, A. P., R. Egli, and B. M. Moskowitz (2007), Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles, J. Geophys. Res., 112,, doi: /2006jb Introduction [2] Firstorder reversal curve (FORC) diagrams are rapidly becoming a useful tool in characterizing rock magnetic properties because they comprehensively incorporate information regarding magnetostatic interactions and domain states. However, a strict quantitative theory of FORC diagrams has not yet been formulated. FORCs are measured by first saturating the sample in a large positive field. The field is then lowered to a reversal field H a. Measurements of magnetization, denoted by M(H a, H b ), are taken at various fields H b as the applied field increases to positive saturation. The FORC function is defined as the mixed second derivative of M(H a, H b )[Mayergoyz, 1986]: rðh a ; H b Þ ¼ 1 2 MH ð a ; H b b which is then plotted on transformed coordinates H c = (H b H a )/2, and H u =(H a + H b )/2 [Pike et al., 1999]. [3] Néel [1954] proposed a simple interpretation of Preisach s [1935] theory for ideal SD grain assemblages, where H c = (H b H a )/2 and H u = (H b + H a )/2 are interpreted as the switching field for an isolated particle 1 Institute for Rock Magnetism and Department of Geology and Geophysics, University of MinnesotaTwin Cities, Minneapolis, Minnesota, USA. Copyright 2007 by the American Geophysical Union /07/2006JB004575$09.00 ð1þ and a bias field related to magnetostatic interactions, respectively. If H c and H u are assumed to be fixed for each grain but different from grain to grain, the FORC function is a Preisach function that can be written as rðh c ; H u Þ ¼ fðh c ÞgH ð u Þ ð2þ where f(h c ) and g(h u ) are the probability density functions (PDFs) of H c and H u, respectively [Pike et al., 1999]. However, the underlying assumption of (2), that H u is constant, is not correct. Furthermore, the hysteresis loop of real SD particles is not rectangular unless a field is applied exactly parallel to particles easy axis. There is an ongoing effort to improve FORC models using more realistic assumptions [e.g., Carvallo et al., 2003; Pike et al., 2005; Newell, 2005; Egli, 2006a]. [4] Deviations of the FORC function from the shape predicted by Preisach models have been repeatedly observed, such as nonelliptical contour lines and negative contributions near the negative H u axis [e.g., Pike et al., 1999; Carvallo et al., 2004]. Mayergoyz [1986] demonstrated that the hysteresis of an assemblage of StonerWohlfarth particles does not obey the congruency property of the Preisach formulism. Newell [2005] calculated the FORC function of noninteracting, randomly oriented Stoner Wohlfarth particles, proving the existence of a negative region and boomerangshaped contour lines in the lower half (H u < 0) of the FORC space. Furthermore, he showed that the FORC function is zero for H u > 0. Both of these results question the possibility of interpreting FORC dia 1of13
2 grams according to equation (2). On the other hand, however, the FORC diagram of real singledomain (SD) particle assemblages shares many common characteristics with the classic Preisach model. For example, measurements [Pike et al., 1999; Carvallo et al., 2005] and numerical models [Muxworthy et al., 2004] of interacting SD particles show that the width of the FORC distribution along H u increases with increasing packing fraction, as predicted by the classic Preisach model. Egli [2006a] developed an exact FORC theory for weakly interacting SD grains. This theory describes a set of magnetic moments whose magnetic coupling is not sufficient to produce a collective behavior; that is, only a very small subset of moments switches in unison. If s i and s c are the typical widths of the interaction field distribution and the switching field distribution, respectively, and m c is the median switching field, a particular result of the dipolar interaction model of Egli [2006a] is valid if s i 2s c and s i 2m c.inthis case, the FORC function is given by the sum of two functions, P and Q, which represent the intrinsic contribution of dipolar interactions and of the reversible component of the hysteresis loop, respectively. As discussed by Newell [2005], the contribution of the reversible component may depend on the switching mode of the particles and is influenced by thermal activation effects. Furthermore, numerical calculations show that Q is negligible close to the main peak of the FORC function near the H c axis, and in the entire upper half of the FORC space [Egli, 2006a]. The component P is given by PH ð c ; H u Þ h# swi w f ð H cþg H u H m ð3þ wh ð c Þ where h# sw i is a constant that depends on the reversible component of the elemental hysteresis loops, H m is the mean interaction field, and 0 w(h c ) 1 is the proportion of all magnetic moments that change reversibly upon cycling from H a to H b, and thus fulfill the assumption of the classic Preisach model [Egli, 2006a]. A firstorder approximation to w(h c ) is given by 1 F(H c ), where FH ð c Þ ¼ Z 1 H c fðhþdh is the cumulative function of f(h c ). Since w is a monotonically decreasing function of H c, the width of P along H u decreases toward the right end of the FORC space, giving to the contour lines of the FORC function a characteristic teardrop shape that have been observed in highly dispersed SD particles [Pike et al., 1999]. The dependence of g(h u /w) on H c is best visualized by the normalized FORC function r* ðh c ; H u Þ ¼ r ð H c; H u Þ max rðh c ; H u Þ H u defined as r(h c, H u ) divided its maximum for every given H c. The contour lines of the normalized FORC function have the same shape as w(h c ) 1 F(H c ). A convergence (divergence) of the contour lines of r* toward large values of H c can be directly interpreted as a thinning (broadening) ð4þ ð5þ of FORC profiles along H u. If r(h c, H u ) is a Preisach function, the contour lines of r* are parallel to the H c axis. [5] The coercivity distribution f(h c ) does not correspond to the intrinsic switching field distribution of noninteracting particles, and is best approximated by the marginal distribution r c ðh c Þ ¼ Z 1 1 rðh c ; H u ÞdH u ð6þ [Winklhofer and Zimanyi, 2006; Egli, 2006a]. In the case of weak interactions, the function g in (3) is identical to the scaled distribution of the local interaction field produced by randomly distributed dipoles: g(h) =W(H; p, zm s, g), with WðH; p; m s ; g e a=b Þ ¼ pb ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi a p p K 1 1 þ H 2 =a 2 b ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi 1 þ H 2 =a 2 where p and m s are the packing fraction and the saturation magnetization of the particles, respectively, a = a 0 (g)pm s, b = b 0 (g)pm s 2 are two constants that depend on the magnetization state and the average alignment g of the dipoles with the applied field, z is a correction factor for the reduction of vector FORC to scalar FORC, and K 1 is the modified Bessel function of the second kind [Egli, 2006a]. The correction factor depends on the reversal mode of the particles: z for StonerWohlfarth particles, and z 1.58 for the curling reversal mode calculated by Aharoni [1999]. Equations (3) (7) provide a quantitative description of the effects of dipolar interaction on the FORC function. [6] In this paper, we present FORC measurements of samples containing magnetosomes, which are characterized by well constrained grain sizes and shapes within the stable SD range. These samples provide the ideal basis to selectively test the dependence of FORC diagrams on the spatial arrangement of the particles. 2. Sample Description and Preparation 2.1. Cultured Magnetite Magnetosomes [7] Cultures of magnetotactic bacteria strains MV1 and MV2 were used to prepare synthetic samples of interacting SD particles. Both MV1 and MV2 produce magnetosomes that are (61 ± 12) (52 ± 11) nm elongated hexagonal prisms of pure magnetite, arranged in a single chain of particles [Meldrum et al., 1993]. The particles are extremely well constrained in size and chemical composition, and fall within the stable singledomain size limit [Butler and Banerjee, 1975; Witt et al., 2005]. MV1 and MV2 were cultured anaerobically in the laboratory from isolated water sample collected in New England, and provided to us by D. Bazylinski (Iowa State University). Details on the culture method are described by Moskowitz et al. [1993]. [8] We prepared two sets of samples: a virtually noninteracting dispersion of intact magnetosome chains still contained within the cells, and disordered assemblages of magnetosomes obtained by destroying the original chain structure through cell rupture. The noninteracting sample, MV1KAOL, was prepared from a fresh aqueous cell suspension by injecting 0.5 ml of the cell suspension into dense slurry of pure kaolin powder (ScienceLab) mixed with distilled water. The mixture was vigorously stirred and ð7þ 2of13
3 then dried at room temperature overnight. The dry product was gently powdered and pressed in a plastic box. Previous measurements of the kaolin powder showed that it was free of ferrimagnetic contaminants. The preparation procedure of this sample was chosen to produce a sample of well dispersed bacterial cells in a clay matrix that mimics dried lake and marine sediments. The saturation magnetization for MV1KAOL is 25 ma m 2 /kg, which is equivalent to a nominal packing fraction (i.e., the volume occupied by the magnetic particles divided by the total volume) of p = The estimated average distance between the magnetosome chains, calculated assuming a typical chain length of 15 magnetosomes, is 6 times the length of a chain. The ratio of the anhysteretic remanent magnetization susceptibility to the isothermal remanent magnetization (ARM ratio) is c ARM /IRM = 2.77 mm/a, in good agreement with results of previous studies on magnetotactic bacteria [Moskowitz et al., 1988, 1993] and with typical values of 2 3 mm/a that characterizes magnetic components of bacterial magnetite in marine and lake sediments [Egli, 2004]. These values are compatible with the theoretical estimates obtained for noninteracting SD magnetite [Egli and Lowrie, 2002]. An additional constraint on the homogeneity of the sample is set by theoretical calculations of the effect of dipole interactions on c ARM /IRM, which shows that dispersed SD magnetite with a packing fraction p <10 4 is not affected by magnetostatic interactions [Egli, 2006b]. [9] Interacting samples of MV1 and MV2 were prepared using magnetosomes extracts obtained with a French press technique [Moskowitz et al., 1993]. The extraction process removes most of the organic material and also destroys the linear chain structure. Freezedried MV1 and MV2 magnetosomes were stored in our laboratory for 7 years and 15 years, respectively. The thermal demagnetization of lowtemperature SIRM for both MV1 and MV2 shows very similar behavior with partially suppressed Verwey transitions indicative of partially oxidized magnetite. [10] Samples MV1GRIDS and MV2GRIDS were prepared by depositing the MV1 and MV2 extracts onto 20 carboncoated Formvar transmission electron microscopy (TEM) copper grids. One MV1 grid and one MV2 grid were randomly selected for electron microscope characterization. The remaining grids were stacked and cemented with Epoxy resin. Each sample consists of a stack of 19 grids holding the extracted MV1 and MV2 magnetosomes, respectively. This preparation method ensured the same arrangement of the particles in the samples prepared for magnetic measurements and the electron microscopy Lake Sediment [11] Lake sediments usually contain a mixture of magnetic minerals of various origins, and a variable amount of fossil magnetosome chains produced by magnetotactic bacteria (magnetofossils). Magnetofossils account typically for 20 60% of the total sediment magnetization [Egli, 2004; Kim et al., 2005]. Egli [2004] reported one case with an unusually high concentration of magnetofossils. The magnetofossils were concentrated in a 5 mm thick organic rest (sample BAIK) embedded in a sediment core retrieved from the deep northern part of lake Baikal (Russia). A detailed coercivity analysis revealed that 93% of the ARM and 76% of the isothermal remanent magnetization of BAIK is carried by two magnetic components that can be attributed to magnetofossils. However, the ARM ratio of these components (c ARM /IRM = 0.07 mm/a) is unusually low, and more than 1 order of magnitude smaller than predicted for SD particles. Egli [2004] formulated a hypothesis for the unusually low ARM ratio of magnetofossils in BAIK and in some other anoxic sediments; however, a definitive explanation was not found. 3. Measurements 3.1. FORC and Hysteresis Measurements [12] The measurement of hysteresis loops and FORC were performed at room temperature using an Alternating Gradient Force Magnetometer (Princeton Measurements Corporation). Hysteresis loops were measured in a maximum field of 500 mt and averaging time of 500 ms. FORC diagrams were obtained from the measurement of 200 partial hysteresis curves using a saturating field of 350 mt and an averaging time of 300 ms. Samples MV1GRIDS and MV2 GRIDS were mounted on the sample holder such that the applied field was parallel to the plane of the grids. Since all samples are magnetically weak, three sets of FORC curves were measured and averaged to increase the signaltonoise ratio Remanence Measurements [13] All samples were initially demagnetized along three perpendicular directions using an alternating field with initial amplitude of 200 mt. ARMs were imparted using a peak alternating field of 200 mt and a 0.1 mt DC bias field. The ARM was measured using a 2G superconducting cryogenic magnetometer Transmission Electron Microscopy [14] Transmission electron microscopy (TEM) was used to obtain a semiquantitative characterization of the geometrical arrangement of the particles in MV1GRIDS and MV2GRIDS, in order to evaluate the interaction field inside the samples. One copper grid from MV1GRIDS and one from MV2GRIDS were selected for examination under a FEI Tecnai 12 transmission electron microscope with 120 kev operating voltage. The grids were mounted on a singletilt specimen holder and the slightly underfocused images were taken using an objective aperture. Two hundred and eightyseven and one hundred and thirtyeight images were captured for MV1GRIDS, and MV2GRIDS, respectively. [15] Unfortunately, it was not possible to obtain TEM images of BAIK or MV1KAOL. Despite the relatively high concentration of magnetic particles, BAIK appeared as a black, homogeneous substance. The minute amount of material remaining from various experiments was not enough to allow a separation of the magnetic carriers from the organic mass. The magnetosomes in MV1KAOL were presumably attached to kaolin particles used to disperse them, and could not be resolved under the microscope. 4. Results and Analysis 4.1. M rs /M s and c ARM /M rs [16] The remanence ratio M rs /M s and the ARM ratio c ARM /M rs for the four samples are reported in Table 1. 3of13
4 Table 1. Sample Description, c ARM /M rs and M rs /M s Ratios of Samples Included in This Study a Sample Description Measured M rs /M s Measured c ARM /M rs 10 3 m/a Predicted c ARM /M rs MV1KAOL whole cell suspension disbursed in kaolin MV1GRIDS extracted magnetosomes deposited on TEM grids glued together by epoxy MV2GRIDS extracted magnetosomes deposited on TEM grids glued together by epoxy BAIK organic rest (from Lake Baikal) b a Predicted values of c ARM /M rs for samples MV1GRIDS and BAIK where obtained using equation (11). b From Egli [2004], calculated from the sum of the two biogenic components. Both the remanence ratio and the ARM ratio of SD particles are lowered by magnetostatic interactions. Muxworthy et al. [2003] used a micromagnetic model to calculate the hysteresis loops of arrays of magnetic particles of various sizes. According to their calculations, the remanence ratio and the coercivity of uniaxial SD particles is unaffected by interactions if the particle spacing d (defined as the distance between the surfaces of two particles, divided by their diameter) is >1. This limit corresponds to a packing fraction p = 0.12 for their cubic particles. On the other hand, ARM is much more sensitive to magnetostatic interactions. Egli [2006b] calculated the factor r i by which the ARM of interacting particles is lowered, with respect to the noninteracting case. For uniaxial SD particles (M rs /M s = 0.5, c ARM /IRM = 2.77 mm/a), r i = 0.95 when p = , and r i = 0.5 when p = Among the four samples, MV1KAOL and BAIK are the only samples displaying the typical M rs /M s ratio of noninteracting uniaxial SD grains (Table 1) TEM Particle Counts [17] Figure 1 shows representative TEM images of MV1 GRIDS and MV2GRIDS. An overall feature of both samples is the existence of groups of closely packed magnetosomes, hereafter referred to as clusters, and of isolated magnetosomes. Intact chains were absent. Whereas the magnetosomes in sample MV2GRIDS are connected by residual organic matter from the cells, particles from MV1GRIDS are almost always in direct contact with one another within a cluster. The residual organic matter in MV2GRIDS prevented the formation of compact clusters of magnetosomes that are in direct contact. [18] We obtained a geometrical characterization of the samples by quantifying the occurrence of clusters and isolated magnetosomes. To do so, we defined a unit as either a cluster or an isolated particle which is at least 3 particle diameters (i.e., nm) away from its nearest neighboring cluster or particle. Magnetosomes attached to large, irregular particles of unknown origin are not used for the counting. The number of magnetosomes in a cluster was determined by direct counting when possible. Magnetosome counts cannot be obtained on large clusters, since they extend into the third dimension forming more than one layer of overlapping particles. In this case, a lower limit for the number of magnetosomes in a cluster was estimated by measuring the area occupied by the cluster (pixel counts). The area was then divided by the averaged projected area of a single magnetosome. Following these procedures, 801 counts from MV1GRIDS and 301 counts from MV2 GRIDS were obtained. We then used these counts to obtain a semiquantitative estimate of the statistical frequency of individual particles and clusters of various sizes (Figure 2). An overall difference between MV1GRIDS and MV2 GRIDS is given by the relative abundance of isolated magnetosomes and small clusters containing up to 20 particles: this category occurs less frequently in MV2GRIDS. On the other hand, there is an overwhelming abundance of large clusters (>300 magnetosomes) in MV2GRIDS FORC Diagrams [19] FORC diagrams were calculated using the FORCO BELLO MATLAB code version 0.99c [Winklhofer and Zimanyi, 2006]. FORC measurements of MV1GRIDS, MV2GRIDS, and BAIK were processed using a smoothing factor SF = 5; SF = 3 was used to process FORC measurements of MV1KAOL. The FORC distributions obtained from multiple measurements of each sample have been averaged to increase the signaltonoise ratio (Figures 3 6). Although all samples are assemblages of magnetosomes with similar intrinsic magnetic properties, the corresponding FORC diagrams display evident differences that are related to the spatial arrangement of the particles. MV1 KAOL is characterized by the simplest FORC function, which consists of a single, narrow peak centered at H c =65 mt (Figure 5). We chose a small smoothing factor (SF = 3) for this sample, which was not sufficient to remove the measurement noise completely, because higher SF values produced an evident broadening of the FORC function. The FORC function of MV1GRIDS is evidently bimodal, with two peaks centered at H c = 30 mt and H c = 52 mt, respectively (Figure 3). The same trend is shown by MV2GRIDS, however, the bimodal nature of the FORC function is much less evident in this case. The FORC distribution of BAIK consists of a single broad peak centered at H c = 56 mt, whereby the nearby elliptic contours indicate that r(h c, H u ) is similar to a Neel s interpretation of Preisach function (Figure 6a). This interpretation is also supported by the weak dependence of the normalized FORC function r*(h c, H u )onh c, unlike the strong H c dependence of r*(h c, H u ) for MV1GRIDS and MV2GRIDS Interpretation of the FORC Diagrams [20] Since all samples presented here are assemblages of almost ideal uniaxial SD particles with various degrees of interactions, we will analyze the FORC diagrams using 4of13
5 [21] In the case of a homogeneous sample of randomly dispersed, SD particles, profiles of the FORC distribution along H u can be modeled using gh ð u Þ ¼ 1 wh ð c Þ W H u H m wh ð c Þ ; p; zm s; g where W is given by equation (7), m s is the saturation magnetization, and H m is a mean interaction field that accounts for a shift of the peak of FORC function peak away from the H c axis. Equation (8) contains five unknown parameters: (1) the packing fraction p, (2) the mean field H m, (3) the function w = w(h c ) with w(0) = 1, (4) the dimensional constant z that depends on the switching mode of the particles, and (5) the average moment alignment g. Only two parameters can be obtained by fitting a FORC profile using (8). If we choose to optimize p and H m, some default values must be assumed for the other parameters. As shown by Egli [2006a], 1.35 z 1.58 depends on the switching model (lower limit corresponds to coherent switching while reversal by curling was used to approximate the upper limit), and w 0.6 at the peak of the distribution. The interaction field distribution is approximately independent of the dipole alignment for p < 0.1, and the solution for random dipoles can be used in this case. Therefore we will use following default parameters: z = 1.354, w 0.6, and g = 0.5. In order to test the validity of this approach, we compare equation (8) with a profile of the FORC function through the peak for a sample of acicular maghemite measured by Carvallo et al. [2004]. Egli [2006a] analyzed this profile using a complete FORC model which was not limited to the case of weak ð8þ Figure 1. (a d) Representative TEM images of sample MV1GRIDS. (e h) Representative TEM images of sample MV2GRIDS. Magnetosomes adhering to irregularly shaped particles of unknown origin, visible on the edges of Figures 1b, 1c, and 1d, were excluded from the counting. Residual organic matter connecting magnetosomes are almost always present in MV2GRIDS but not in MV1GRIDS. In Figure 1c, examples of three different arrangements of paired magnetosome are highlighted: (1) sidebyside, (2) headtohead, and (3) an intermediate configuration. equations (3) (7). We are particularly interested in the possibility of gaining information about the effective concentration of magnetic particles, and in checking the compatibility of results obtained from FORC measurements with constraints set by other measurements, such as ARM. Figure 2. Histogram of cluster sizes for MV1GRIDS and MV2GRIDS. The counts are assigned into log scale bins, and the volume occupied by each bin is shown as a fraction of the total volume counted for the sample. Large clusters are relatively more abundant in MV2GRIDS, whereas individual magnetosomes as well as smaller clusters are more common in MV1GRIDS than in MV2GRIDS. Histograms are based on 801 counts from MV1GRIDS and 301 counts from MV2GRIDS. 5of13
6
7 7 of 13
8 5. Discussion 5.1. Strong Positive Interactions in Magnetosome Chains and FORC Diagrams [27] A positive or negative interaction field is defined by its direction relative to the sample's magnetization vector. Positive and negative interaction fields cancel out statistically in an isotropic sample, and the local interaction field is described by a statistical variate with zero mean [Shcherbakov and Shcherbakova, 1975]. In anisotropic samples, however, the average local interaction field H m can be different from zero. Chains of magnetic particles are expected to be dominated by positive interactions, whence
9 switch their moment in unison at a critical external field. A vertical spread on the order of 20 mt has been observed in FORC diagrams of uncultured magnetotactic bacteria [Pan et al, 2005]. The authors attributed this spread to interchain interaction rather than intrachain interaction. Our FORC observation of MV1KAOL corroborated these previous findings, confirming that each chain acts as an individual SD particle and the FORC does not map strong intrachain interaction FORC Diagrams and Particle Clusters [29] Why is the FORC diagram of almost identical particles bimodal? MV1GRIDS and MV2GRIDS are examples of the complex effects of the geometrical arrangement of the particles on the magnetic properties. Since both 9 of 13
10 Figure 7. Comparison of a profile of the FORC diagram through the peak for acicular maghemite measured by Carvallo et al. [2004] (solid line) with a detailed model described by Egli [2006b] (dots), and a best fit obtained using equation (8) (dashed line). Notice that the detailed model, unlike equation (8), fits the asymmetry of the measured curve. However, both the detailed model and the fit using equation (8) predict the same value for the packing fraction. samples are made of the same particles with strictly controlled dimensions and shapes, differences in their FORC distributions are closely related to their geometrical arrangement. The FORC diagram of MV1GRIDS suggests the existence of two subsets of the sample with different magnetic properties that we interpret as two components with different packing densities. There is no obvious correlation between the existence of two magnetic components and our TEM observations: we observed clusters formed by a number of particles ranging from 1 to several hundreds, without evidence for a bimodal contribution of these clusters to the total volume of the particles (Figure 2). However, the magnetic contribution of each cluster does not correspond to its volume contribution. To better understand the relationship between TEM observations (Figure 1) and the FORC distribution (Figure 3), we hypothesize that the magnetic component with higher coercivity and lower apparent packing fraction is made of individual magnetosomes or small clusters with M rs /M s 0.5. According to the model summarized in Table 3, this component contributes 13% of the total remanent magnetization of MV1GRIDS. Using M rs /M s 0.5, we estimate that the contribution to the total M s is only 6.7%. Since M s is proportional to the volume, this magnetic component contributes to 6.7% of the total volume of the particles. From TEM observations we know that the volume contribution of isolated magnetosomes is 4.4%, followed by 3.8% of magnetosome pairs. Observed pairs of magnetosomes had headtohead, sidebyside, or intermediate configurations (Figure 1c). The sidebyside arrangement produces a stable magnetic configuration with a zero net magnetic moment, whereas the headtohead arrangement is equivalent to a chain of two magnetosomes with SD behavior. By assuming that 50% of the magnetosome pairs have SD behavior, we estimate that 6.3% of the volume of the observed particles contributes to the highcoercivity FORC component. This estimate is close to the 6.7% determined from the FORC diagram. We therefore conclude that the bimodal character of the FORC diagram reflects an important difference between the magnetic properties of isolated (and some pairs) of particles on one hand, and clusters on the other. Compared to MV1 GRIDS, the FORC diagram of MV2GRIDS shows little evidence of a component characterized by the high coercivity of noninteracting magnetosomes. This is to some extent due to the smaller number of isolated and paired particles in MV2GRIDS (Figure 2). [30] Another difference between the FORC distribution of MV1GRIDS and MV2GRIDS is the apparent packing fraction of the magnetic component related to the particle clusters: p = 0.20 in MV1GRIDS, and p = 0.08 in MV2 GRIDS. The packing fractions correspond to a difference of 33% in the average separation of the particles each cluster. TEM images confirm this difference: clusters in MV2 GRIDS contain magnetosomes that are separated by organic matter residuals (Figure 1). [31] A difference of 53% is observed between the apparent coercivity of the two components of the FORC Table 2. Summary of Least Squares Fitting Parameters of Selected FORC Profiles, Obtained Using Equation (9) a Sample H c,mt Magnetic Contribution a (Arbitrary Units) Packing Fraction p, % H m,mt MV1GRIDS ± ± ± ± ± ± ± ± ± ± ± ± 1 MV2GRIDS ± ± ± ± ± ± ± ± ± 0.05 MV1KAOL ± ± ± 0.1 BAIK ± ± ± ± ± ± 0.04 a Dashed lines in Figures of 13
11 difference between the magnetosomes in the two samples, which were prepared from different bacterial cultures [Moskowitz et al, 1993] Negative Contributions to the FORC Function [33] Despite the theoretical predictions of Newell [2005] and experimental observations [Pike et al, 1999; Carvallo et al, 2004], all FORC functions presented in this paper are positive over the entire FORC space. We did not observe the "negative region" predicted for StonerWohlfarth particles or by the moving Preisach model [Pike et al, 1999]. Thermal activations are also affecting the reversal mode, as discussed by Newell [2005]. Finally, the situation is complicated by the fact that the magnetosomes in MV1 GRIDS and MV2GRIDS are partially oxidized, whereby the existence of an oxidation gradient has unknown effects on the angular dependence of the anisotropy energy of the particles. Factors such as the width of particle size distribution and the aspect ratio may also be related to the lack of negative contributions in MV1GRIDS and MV2GRIDS, compared to the FORC diagram of acicular maghemite [Carvallo et al, 2004]. [34] Our observations demonstrate that features of the FORC diagram related to the reversible magnetization of SD particles are difficult to model, since they depend Figure 8. A model of the FORC diagram of MV1GRIDS using two components defined by equation (12). (a) FORC function of component 1. (b) FORC function of component 2. (c) Sum of the two components, (d) Square fitting residuals between Figure 8c and the measured FORC diagram of MV1GRIDS (Figure 3). Figures 8c and 8d have the same color scale. 11 of 13
12 critically on a detailed micromagnetic knowledge of the magnetic behavior of the particles Interactions in Natural Sediments [35] The extraordinary uniformity of magnetosomes allows us to use the results obtained with our samples to understand the arrangement of authigenic magnetic particles in natural sediments. As shown by the BAIK sample, the existence of different magnetic components imply a complex spatial relationship of the magnetic particles. Particles belonging to the same component may occur in isolated clusters, whereby dipolar interactions between particles of the same component are probably stronger than interactions between different components. This explains the observed linear additivity of magnetic components [e.g., Carter Stiglitz et al., 2001; Kruiver et al., 2001; Egli, 2004], as well as the fact that FORC diagrams of natural samples are generally closer to a Preisach function than synthetic samples. [36] FORC diagrams of natural samples show a variety of features that requires an intensive modeling effort to be fully understood [Roberts et al., 2000]. The example of BAIK shows that FORC diagrams can be used successfully to model the effect of dipolar interaction on the magnetic properties of known magnetic components. This is especially useful for such magnetic properties that are extremely sensitive to interactions, such as the ARM. As demonstrated by Egli [2004], ARM measurements are better suited to the identification of authigenic components in sediments, however, the interpretation depends on the presence of interactions. The comparison of c ARM /M rs of authigenic components with the values predicted for noninteracting SD particles by Egli and Lowrie [2002], together with the predicted onset of significant interaction effects at p >10 3 [Egli, 2006b], indicates that the magnetic particles are generally extremely well dispersed in sediments. While this can be expected of the case intact chains of magnetosomes, it is not obviously true of other magnetic components, which are not surrounded by cell material that prevents aggregation. However, a generalization of this observation should be considered carefully, as demonstrated by the strong interaction effects observed in BAIK. 6. Conclusion [37] We demonstrated that a quantitative interpretation of FORC measurements of interacting SD particles is possible. A comparison of the FORC function with the distribution of local interaction fields predicted by theoretical models provides a rough estimate of the effective packing fraction of SD magnetic particles. Since the particles have similar magnetic properties, we were able to isolate the effects of spatial arrangements and show that they have a strong effect on the FORC function. For example, we observed a clearly bimodal FORC distribution on synthetic samples containing magnetosomes arranged in clusters of various sizes ranging from a single particle to several hundreds. The estimate of the particle concentration obtained from FORC measurements was used to calculate the effect of magnetostatic interactions on the ARM. The calculated effect is in excellent agreement with measurements, demonstrating the validity of quantitative theories of dipolar interactions. [38] Acknowledgments. We thank Dennis Bazylinski for providing us with samples of magnetotactic bacteria. We also want to thank Michael Winklhofer and Andrew Newell for providing detailed comments that led to significant improvements in the original manuscript. Amy P. Chen was supported by the University of Minnesota s Undergraduate Research Opportunities Program (UROP). The Institute for Rock Magnetism is supported by a grant from the Instruments and Facilities Program, Earth Science Division, the National Science Foundation. This is IRM contribution References Aharoni, A. (1999), Curling reversal mode in nonellipsoidal ferromagnetic particles, J. Appl. Phys., 86, Butler, R. F., and S. K. Banerjee (1975), Theoretical singledomain grainsize range in magnetite and titanomagnetite, J. Geophys. Res., 80, CarterStiglitz, B., B. Moskowitz, and M. Jackson (2001), Unmixing magnetic assemblages and the magnetic behavior of bimodal mixtures, J. Geophys. Res., 106, 26,397 26,411. Carvallo, C., A. R. Muxworthy, D. J. Dunlop, and W. Williams (2003), Micromagnetic modeling of firstorder reversal curve (FORC) diagrams for singledomain and pseudosingledomain magnetite, Earth Planet. Sci. Lett., 213, Carvallo, C., Ö. Özdemir, and D. J. Dunlop (2004), Firstorder reversal curve (FORC) diagrams of elongated singledomain grains at high and low temperatures, J. Geophys. Res., 109, B04105, doi: / 2003JB Carvallo, C., D. Dunlop, and Ö. Özdemir (2005), Experimental comparison of FORC and remanent Preisach diagrams, Geophys. J. Int., 162, Egli, R. (2004), Characterization of individual rock magnetic components by analysis of remanence curves. 1. Unmixing natural sediments, Stud. Geophys. Geodaet., 48, Egli, R. (2006a), Theoretical aspects of dipolar interactions and their appearance in firstorder reversal curves of thermally activated singledomain particles, J. Geophys. Res., 111, B12S17, doi: /2006jb Egli, R. (2006b), Theoretical considerations on the anhysteretic remanent magnetization of interacting particles with uniaxial anisotropy, J. Geophys. Res., 111, B12S18, doi: /2006jb Egli, R., and W. Lowrie (2002), Anhysteretic remanent magnetization of fine magnetic particles, J. Geophys. Res., 107(B10), 2209, doi: / 2001JB Kim, B. Y., K. P. Kodama, and R. E. Moeller (2005), Bacterial magnetite produced in water column dominates lake sediment mineral magnetism: Lake Ely, USA, Geophys. J. Int., 163, Kruiver, P. P., M. J. Dekkers, and D. Heslop (2001), Quantification of magnetic coercivity components by the analysis of acquisition curves of isothermal remanent magnetization, Earth Planet. Sci. Lett., 189, Mayergoyz, I. D. (1986), Mathematical models of hysteresis, Phys. Rev. Lett., 56, Meldrum, F. C., S. Mann, B. R. Heywood, R. B. Frankel, and D. A. Bazylinski (1993), Electron microscopy study of magnetosomes in two cultured vibrioid magnetotactic bacteria, Proc. R. Soc. London, Ser. B, 251, Moskowitz, B., R. Frankel, P. Flanders, R. Blakemore, and B. Schwartz (1988), Magnetic properties of magnetotactic bacteria, J. Magn. Magn. Mater., 73, Moskowitz, B. M., R. B. Frankel, and D. A. Bazylinski (1993), Rock magnetic criteria for the detection of biogenic magnetite, Earth Planet. Sci. Lett., 120, Muxworthy, A., W. Williams, and D. Virdee (2003), Effect of magnetostatic interactions on the hysteresis parameters of singledomain and pseudosingledomain grains, J. Geophys. Res., 108(B11), 2517, doi: / 2003JB Muxworthy, A. R., D. Heslop, and W. Williams (2004), Influence of magnetostatic interactions on firstorderreversalcurve (FORC) diagrams a micromagnetic approach, Geophys. J. Int., 158, Néel, L. (1954), Remarques sur la théorie des propriétés magnétiques des substances dures, Appl. Sci. Res., B4, Newell, A. J. (2005), A highprecision model of firstorder reversal curve (FORC) functions for singledomain ferromagnets with uniaxial anisotropy, Geochem. Geophys. Geosyst., 6, Q05010, doi: / 2004GC Pan, Y., N. Petersen, M. Winklhofer, A. F. Davila, Q. Liu, T. Frederichs, M. Hanzlik, and R. Zhu (2005), Rock magnetic properties of uncultured magnetotactic bacteria, Earth Planet. Sci. Lett., 237, Penninga, I., H. D. Waard, B. M. Moskowitz, D. A. Bazylinski, and R. B. Frankel (1995), Remanence measurements on individual magnetotactic 12 of 13
13 bacteria using a pulsed magnetic field, J. Magn. Magn. Mater., 149, Pike, C. R., A. P. Roberts, and K. L. Verosub (1999), Characterizing interactions in fine magnetic particle system using first order reversal curves, J. Appl. Phys., 85, Pike, C. R., C. A. Ross, R. T. Scalettar, and G. Zimanyi (2005), Firstorder reversal curve diagram analysis of a perpendicular nickel nanopillar array, Phys. Rev. B, 71, Preisach, F. (1935), Uber die magnetische Nachwirkung, Z. Phys., 94, Roberts, A. P., C. R. Pike, and K. L. Verosub (2000), FORC diagram: A new tool for characterizing the magnetic properties of natural samples, J. Geophys. Res., 105, 28,461 28,475. Shcherbakov, V. P., and V. Shcherbakova (1975), On the magnetostatic interaction in a system of singledomain grains, Izv. Earth Phys., 9, Winklhofer, M., and G. T. Zimanyi (2006), Extracting the intrinsic switching field distribution in perpendicular media: A comparative analysis, J. Appl. Phys., 99, 08E710, doi: / Witt, A., K. Fabian, and U. Bleil (2005), Threedimensional micromagnetic calculations for naturally shaped magnetite: Octahedra and magnetosomes, Earth and Planet. Sci. Lett., 233, A. P. Chen, R. Egli, and B. M. Moskowitz, Institute for Rock Magnetism and Department of Geology and Geophysics, University of Minnesota, Minneapolis, MN 55455, USA. 13 of 13
FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS
FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS Adrian R. Muxworthy* and Andrew P. Roberts School of Ocean and Earth Science, National Oceanography Centre, European Way, University of Southampton, Southampton,
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationPreisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective
Preisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective R M. Roshko Department of Physics and Astronomy University of Manitoba Winnipeg, Manitoba, Canada First Order Reversal
More informationMagnetic Media Measurements with a VSM
Magnetic Media Measurements with a VSM B. C. Dodrill Lake Shore Cryotronics, Inc. 575 McCorkle Blvd Westerville, Ohio 43082 The last 50 years have seen the development of methods for the digital storage
More informationNew Approach to Analysis of the Switching Current Data in Ferroelectric Thin Films
Ferroelectrics, 291: 27 35, 2003 Copyright c Taylor & Francis Inc. ISSN: 00150193 print / 15635112 online DOI: 10.1080/00150190390222510 New Approach to Analysis of the Switching Current Data in Ferroelectric
More informationAnomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films
Anomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films J. R. Lindemuth a, B. C. Dodrill a and N. C. Oldham b a Lake Shore Cryotronics, Inc. 575 McCorkle Blvd,
More informationEXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION
EXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION Hua Yuan and David E. Laughlin Department of Materials Science and Engineering, Carnegie Mellon
More informationData Exploration Data Visualization
Data Exploration Data Visualization What is data exploration? A preliminary exploration of the data to better understand its characteristics. Key motivations of data exploration include Helping to select
More informationDemographics of Atlanta, Georgia:
Demographics of Atlanta, Georgia: A Visual Analysis of the 2000 and 2010 Census Data 36315 Final Project Rachel Cohen, Kathryn McKeough, Minnar Xie & David Zimmerman Ethnicities of Atlanta Figure 1: From
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationIncorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
The OpenAccess Journal for the Basic Principles of Diffusion Theory, Experiment and Application Incorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationEM4: Magnetic Hysteresis
CHALMERS UNIVERSITY OF TECHNOLOGY GÖTEBORG UNIVERSITY EM4: Magnetic Hysteresis Lab manual (version 1.001a) Students:... &... Date:... /... /... Laboration passed:... Supervisor:... Date:... /... /... Raluca
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationExploratory data analysis (Chapter 2) Fall 2011
Exploratory data analysis (Chapter 2) Fall 2011 Data Examples Example 1: Survey Data 1 Data collected from a Stat 371 class in Fall 2005 2 They answered questions about their: gender, major, year in school,
More informationPerformance Level Descriptors Grade 6 Mathematics
Performance Level Descriptors Grade 6 Mathematics Multiplying and Dividing with Fractions 6.NS.12 Grade 6 Math : SubClaim A The student solves problems involving the Major Content for grade/course with
More informationThe accurate calibration of all detectors is crucial for the subsequent data
Chapter 4 Calibration The accurate calibration of all detectors is crucial for the subsequent data analysis. The stability of the gain and offset for energy and time calibration of all detectors involved
More informationAMARILLO BY MORNING: DATA VISUALIZATION IN GEOSTATISTICS
AMARILLO BY MORNING: DATA VISUALIZATION IN GEOSTATISTICS William V. Harper 1 and Isobel Clark 2 1 Otterbein College, United States of America 2 Alloa Business Centre, United Kingdom wharper@otterbein.edu
More informationMarketing Mix Modelling and Big Data P. M Cain
1) Introduction Marketing Mix Modelling and Big Data P. M Cain Big data is generally defined in terms of the volume and variety of structured and unstructured information. Whereas structured data is stored
More informationFall 12 PHY 122 Homework Solutions #8
Fall 12 PHY 122 Homework Solutions #8 Chapter 27 Problem 22 An electron moves with velocity v= (7.0i  6.0j)10 4 m/s in a magnetic field B= (0.80i + 0.60j)T. Determine the magnitude and direction of the
More informationKNOWLEDGE BASE ARTICLE Zero Voltage Transmission (ZVT) Technology. Basics of the GPZ 7000 Technology: Zero Voltage Transmission (ZVT)
KNOWLEDGE BASE ARTICLE Zero Voltage Transmission (ZVT) Technology Basics of the GPZ 7000 Technology: Zero Voltage Transmission (ZVT) By Bruce Candy Basic Metal Detection Principles 1 2 3 4 Simplified representation
More informationNonlinear Iterative Partial Least Squares Method
Numerical Methods for Determining Principal Component Analysis Abstract Factors Béchu, S., RichardPlouet, M., Fernandez, V., Walton, J., and Fairley, N. (2016) Developments in numerical treatments for
More informationThe Olympus stereology system. The Computer Assisted Stereological Toolbox
The Olympus stereology system The Computer Assisted Stereological Toolbox CAST is a Computer Assisted Stereological Toolbox for PCs running Microsoft Windows TM. CAST is an interactive, userfriendly,
More informationDESCRIPTIVE STATISTICS. The purpose of statistics is to condense raw data to make it easier to answer specific questions; test hypotheses.
DESCRIPTIVE STATISTICS The purpose of statistics is to condense raw data to make it easier to answer specific questions; test hypotheses. DESCRIPTIVE VS. INFERENTIAL STATISTICS Descriptive To organize,
More information3211 Ferromagnetism Ferromagnetic material having strong permanent magnetism Diamagnetic or paramagnetic material having weak
3211 Ferromagnetism Ferromagnetic material having strong permanent magnetism Diamagnetic or paramagnetic material having weak temporary magnetism. Iron, cobalt, nickel, gadolinium, dysprosium exhibit
More informationLecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe.
Lecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe. Brief Overview of STM Inventors of STM The Nobel Prize in Physics 1986 Nobel
More informationPhysics 221 Experiment 5: Magnetic Fields
Physics 221 Experiment 5: Magnetic Fields August 25, 2007 ntroduction This experiment will examine the properties of magnetic fields. Magnetic fields can be created in a variety of ways, and are also found
More informationCHAPTER4 GENERAL ASPECTS OF MUTUAL
CHAPTER4 GENERAL ASPECTS OF MUTUAL ADMITTANCE OF CPWFED TWIN SLOTS ON CONDUCTORBACKED TWOLAYER SUBSTRATES 4.1 INTRODUCTORY REMARKS The present chapter is concerned with an exploratory investigation
More informationPPT No. 26. Uniformly Magnetized Sphere in the External Magnetic Field. Electromagnets
PPT No. 26 Uniformly Magnetized Sphere in the External Magnetic Field Electromagnets Uniformly magnetized sphere in external magnetic field The Topic Uniformly magnetized sphere in external magnetic field,
More informationChapter 7: Polarization
Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces
More informationEE ELECTRICAL MATERIAL SCIENCE
EE09 506 ELECTRICAL MATERIAL SCIENCE Module I Hard and soft magnetic materials and applications  Ferrites  Magnetic materials used in electrical machines, instruments and relays Arun Xavier VAST 2 Module
More informationIN current film media, the increase in areal density has
IEEE TRANSACTIONS ON MAGNETICS, VOL. 44, NO. 1, JANUARY 2008 193 A New Read Channel Model for Patterned Media Storage Seyhan Karakulak, Paul H. Siegel, Fellow, IEEE, Jack K. Wolf, Life Fellow, IEEE, and
More information15.062 Data Mining: Algorithms and Applications Matrix Math Review
.6 Data Mining: Algorithms and Applications Matrix Math Review The purpose of this document is to give a brief review of selected linear algebra concepts that will be useful for the course and to develop
More informationData Mining: Exploring Data. Lecture Notes for Chapter 3. Slides by Tan, Steinbach, Kumar adapted by Michael Hahsler
Data Mining: Exploring Data Lecture Notes for Chapter 3 Slides by Tan, Steinbach, Kumar adapted by Michael Hahsler Topics Exploratory Data Analysis Summary Statistics Visualization What is data exploration?
More information1. Fluids Mechanics and Fluid Properties. 1.1 Objectives of this section. 1.2 Fluids
1. Fluids Mechanics and Fluid Properties What is fluid mechanics? As its name suggests it is the branch of applied mechanics concerned with the statics and dynamics of fluids  both liquids and gases.
More informationInterpreting Data in Normal Distributions
Interpreting Data in Normal Distributions This curve is kind of a big deal. It shows the distribution of a set of test scores, the results of rolling a die a million times, the heights of people on Earth,
More informationMagnetic Data Storage and Nanoparticles Ernie Chang
Magnetic Data Storage and Nanoparticles Ernie Chang Introduction Magnetic storage, specifically in hard drives has advanced significantly since the first disk drive built in 1956 [1]. Interestingly enough,
More informationCommon Core Unit Summary Grades 6 to 8
Common Core Unit Summary Grades 6 to 8 Grade 8: Unit 1: Congruence and Similarity 8G18G5 rotations reflections and translations,( RRT=congruence) understand congruence of 2 d figures after RRT Dilations
More informationEffect of coupling strength on magnetic properties of exchange spring magnets
OURNAL OF APPLIED PHYSICS VOLUME 94, NUMBER 10 15 NOVEMBER 2003 Effect of coupling strength on magnetic properties of exchange spring magnets Vamsi M. Chakka, Z. S. Shan a), and. P. Liu b) Department of
More informationMultivariate Analysis of Ecological Data
Multivariate Analysis of Ecological Data MICHAEL GREENACRE Professor of Statistics at the Pompeu Fabra University in Barcelona, Spain RAUL PRIMICERIO Associate Professor of Ecology, Evolutionary Biology
More informationIris Sample Data Set. Basic Visualization Techniques: Charts, Graphs and Maps. Summary Statistics. Frequency and Mode
Iris Sample Data Set Basic Visualization Techniques: Charts, Graphs and Maps CS598 Information Visualization Spring 2010 Many of the exploratory data techniques are illustrated with the Iris Plant data
More information2D Magnetic Circuit Analysis for a Permanent Magnet Used in Laser Ablation Plume Expansion Experiments
University of California, San Diego UCSDLPLM0204 2D Magnetic Circuit Analysis for a Permanent Magnet Used in Laser Ablation Plume Expansion Experiments Xueren Wang, Mark Tillack and S. S. Harilal December
More informationGlobal Seasonal Phase Lag between Solar Heating and Surface Temperature
Global Seasonal Phase Lag between Solar Heating and Surface Temperature Summer REU Program Professor Tom Witten By Abstract There is a seasonal phase lag between solar heating from the sun and the surface
More information* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B. PPT No.
* Biot Savart s Law Statement, Proof Applications of Biot Savart s Law * Magnetic Field Intensity H * Divergence of B * Curl of B PPT No. 17 Biot Savart s Law A straight infinitely long wire is carrying
More informationFerromagnetic resonance imaging of Co films using magnetic resonance force microscopy
Ferromagnetic resonance imaging of Co films using magnetic resonance force microscopy B. J. Suh, P. C. Hammel, a) and Z. Zhang Condensed Matter and Thermal Physics, Los Alamos National Laboratory, Los
More informationKOLEKTOR MAGNET TECHNOLOGY
ZIT S KOERZIT S Sintered AlNiCo Koerzit is the KOLEKTOR MAGNET TECHNOLOGY GmbH tradename for sintered permanent magnets based on AlNi and AlNiCo alloys. Koerzit magnets are made by powder metallurgy. KOLEKTOR
More informationMeasuring Line Edge Roughness: Fluctuations in Uncertainty
Tutor6.doc: Version 5/6/08 T h e L i t h o g r a p h y E x p e r t (August 008) Measuring Line Edge Roughness: Fluctuations in Uncertainty Line edge roughness () is the deviation of a feature edge (as
More informationModule 1 : Conduction. Lecture 5 : 1D conduction example problems. 2D conduction
Module 1 : Conduction Lecture 5 : 1D conduction example problems. 2D conduction Objectives In this class: An example of optimization for insulation thickness is solved. The 1D conduction is considered
More informationNEW MEXICO Grade 6 MATHEMATICS STANDARDS
PROCESS STANDARDS To help New Mexico students achieve the Content Standards enumerated below, teachers are encouraged to base instruction on the following Process Standards: Problem Solving Build new mathematical
More informationGeography 4203 / 5203. GIS Modeling. Class (Block) 9: Variogram & Kriging
Geography 4203 / 5203 GIS Modeling Class (Block) 9: Variogram & Kriging Some Updates Today class + one proposal presentation Feb 22 Proposal Presentations Feb 25 Readings discussion (Interpolation) Last
More informationAN INVESTIGATION INTO THE USEFULNESS OF THE ISOCS MATHEMATICAL EFFICIENCY CALIBRATION FOR LARGE RECTANGULAR 3 x5 x16 NAI DETECTORS
AN INVESTIGATION INTO THE USEFULNESS OF THE ISOCS MATHEMATICAL EFFICIENCY CALIBRATION FOR LARGE RECTANGULAR 3 x5 x16 NAI DETECTORS Frazier L. Bronson CHP Canberra Industries, Inc. 800 Research Parkway,
More informationPART I SIEVE ANALYSIS OF MATERIAL RETAINED ON THE 425 M (NO. 40) SIEVE
Test Procedure for PARTICLE SIZE ANALYSIS OF SOILS TxDOT Designation: Tex110E Effective Date: August 1999 1. SCOPE 1.1 This method covers the quantitative determination of the distribution of particle
More informationLECTURE #7: MAGNETIC PROPERTIES OF MATERIALS. Basic question: Why are some solids magnetic while others are not?
LECTURE #7: MAGNETIC PROPERTIES OF MATERIALS Basic question: Why are some solids magnetic while others are not? The answers are linked to: Origin of magnetism Types of magnetic materials considered Effects
More informationManual for simulation of EB processing. Software ModeRTL
1 Manual for simulation of EB processing Software ModeRTL How to get results. Software ModeRTL. Software ModeRTL consists of five thematic modules and service blocks. (See Fig.1). Analytic module is intended
More informationMagnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types
Magnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types Identification of magnetic minerals and phases Grain size assessment
More informationPhysical & Chemical Properties. Properties
Physical & Chemical Properties Properties Carbon black can be broadly defined as very fine particulate aggregates of carbon possessing an amorphous quasigraphitic molecular structure. The most significant
More informationSummarizing and Displaying Categorical Data
Summarizing and Displaying Categorical Data Categorical data can be summarized in a frequency distribution which counts the number of cases, or frequency, that fall into each category, or a relative frequency
More informationComposite Electromagnetic Wave Absorber Made of Permalloy or Sendust and Effect of Sendust Particle Size on Absorption Characteristics
PIERS ONLINE, VOL. 4, NO. 8, 2008 846 Composite Electromagnetic Wave Absorber Made of Permalloy or Sendust and Effect of Sendust Particle Size on Absorption Characteristics K. Sakai, Y. Wada, and S. Yoshikado
More informationPrentice Hall Mathematics Courses 13 Common Core Edition 2013
A Correlation of Prentice Hall Mathematics Courses 13 Common Core Edition 2013 to the Topics & Lessons of Pearson A Correlation of Courses 1, 2 and 3, Common Core Introduction This document demonstrates
More informationMEASURES OF CENTER AND SPREAD MEASURES OF CENTER 11/20/2014. What is a measure of center? a value at the center or middle of a data set
MEASURES OF CENTER AND SPREAD Mean and Median MEASURES OF CENTER What is a measure of center? a value at the center or middle of a data set Several different ways to determine the center: Mode Median Mean
More informationMesh Moving Techniques for FluidStructure Interactions With Large Displacements
K. Stein Department of Physics, Bethel College, St. Paul, MN 55112 T. Tezduyar Mechanical Engineering, Rice University, MS 321, Houston, TX 77005 R. Benney Natick Soldier Center, Natick, MA 01760 Mesh
More informationCOM CO P 5318 Da t Da a t Explora Explor t a ion and Analysis y Chapte Chapt r e 3
COMP 5318 Data Exploration and Analysis Chapter 3 What is data exploration? A preliminary exploration of the data to better understand its characteristics. Key motivations of data exploration include Helping
More information2. Simple Linear Regression
Research methods  II 3 2. Simple Linear Regression Simple linear regression is a technique in parametric statistics that is commonly used for analyzing mean response of a variable Y which changes according
More informationE. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE
E. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE References for Nuclear Magnetic Resonance 1. Slichter, Principles of Magnetic Resonance, Harper and Row, 1963. chapter
More informationMultivariate Normal Distribution
Multivariate Normal Distribution Lecture 4 July 21, 2011 Advanced Multivariate Statistical Methods ICPSR Summer Session #2 Lecture #47/21/2011 Slide 1 of 41 Last Time Matrices and vectors Eigenvalues
More informationInsertion Devices Lecture 4 Permanent Magnet Undulators. Jim Clarke ASTeC Daresbury Laboratory
Insertion Devices Lecture 4 Permanent Magnet Undulators Jim Clarke ASTeC Daresbury Laboratory Introduction to Lecture 4 So far we have discussed at length what the properties of SR are, when it is generated,
More informationVALIDATION OF ANALYTICAL PROCEDURES: TEXT AND METHODOLOGY Q2(R1)
INTERNATIONAL CONFERENCE ON HARMONISATION OF TECHNICAL REQUIREMENTS FOR REGISTRATION OF PHARMACEUTICALS FOR HUMAN USE ICH HARMONISED TRIPARTITE GUIDELINE VALIDATION OF ANALYTICAL PROCEDURES: TEXT AND METHODOLOGY
More informationStatistical Study of Magnetic Reconnection in the Solar Wind
WDS'13 Proceedings of Contributed Papers, Part II, 7 12, 2013. ISBN 9788073782511 MATFYZPRESS Statistical Study of Magnetic Reconnection in the Solar Wind J. Enžl, L. Přech, J. Šafránková, and Z. Němeček
More informationLocal outlier detection in data forensics: data mining approach to flag unusual schools
Local outlier detection in data forensics: data mining approach to flag unusual schools Mayuko Simon Data Recognition Corporation Paper presented at the 2012 Conference on Statistical Detection of Potential
More informationT = 1 f. Phase. Measure of relative position in time within a single period of a signal For a periodic signal f(t), phase is fractional part t p
Data Transmission Concepts and terminology Transmission terminology Transmission from transmitter to receiver goes over some transmission medium using electromagnetic waves Guided media. Waves are guided
More informationExploratory Data Analysis
Exploratory Data Analysis Johannes Schauer johannes.schauer@tugraz.at Institute of Statistics Graz University of Technology Steyrergasse 17/IV, 8010 Graz www.statistics.tugraz.at February 12, 2008 Introduction
More informationDiagrams and Graphs of Statistical Data
Diagrams and Graphs of Statistical Data One of the most effective and interesting alternative way in which a statistical data may be presented is through diagrams and graphs. There are several ways in
More informationChapter Test B. Chapter: Measurements and Calculations
Assessment Chapter Test B Chapter: Measurements and Calculations PART I In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question. 1.
More informationGuidance for Industry
Guidance for Industry Q2B Validation of Analytical Procedures: Methodology November 1996 ICH Guidance for Industry Q2B Validation of Analytical Procedures: Methodology Additional copies are available from:
More informationNEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS
NEW YORK STATE TEACHER CERTIFICATION EXAMINATIONS TEST DESIGN AND FRAMEWORK September 2014 Authorized for Distribution by the New York State Education Department This test design and framework document
More informationPOWDER PROPERTIES LABORATORY
Ground Rules POWDER PROPERTIES LABORATORY You will work as a team of no more than 6 students. At the end of this laboratory session each team will turn in a single report. The report will be reviewed,
More informationPHYS 39a Lab 3: Microscope Optics
PHYS 39a Lab 3: Microscope Optics Trevor Kafka December 15, 2014 Abstract In this lab task, we sought to use critical illumination and Köhler illumination techniques to view the image of a 1000 linesperinch
More informationNuclear Magnetic Resonance
Nuclear Magnetic Resonance Introduction Atomic magnetism Nuclear magnetic resonance refers to the behaviour of atomic nuclei in the presence of a magnetic field. The first principle required to understand
More informationExperimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION ( )
a. Using Faraday s law: Experimental Question 1: Levitation of Conductors in an Oscillating Magnetic Field SOLUTION The overall sign will not be graded. For the current, we use the extensive hints in the
More informationIn mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data.
MATHEMATICS: THE LEVEL DESCRIPTIONS In mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data. Attainment target
More informationPermanent Magnet Materials
Measurements with a VSM Permanent Magnet Materials B. C. Dodrill B. J. Kelley Lake Shore Cryotronics, Inc. 575 McCorkle Blvd. Westerville, OH, 43082 Please address correspondence to bdodrill@lakeshore.com
More informationMultiple Optimization Using the JMP Statistical Software Kodak Research Conference May 9, 2005
Multiple Optimization Using the JMP Statistical Software Kodak Research Conference May 9, 2005 Philip J. Ramsey, Ph.D., Mia L. Stephens, MS, Marie Gaudard, Ph.D. North Haven Group, http://www.northhavengroup.com/
More informationEtudes in situ et ex situ de multicouches C/FePt
Etudes in situ et ex situ de multicouches C/FePt : influence de la température sur la structure et les propriétés s magnétiques D. Babonneau, G. Abadias, F. Pailloux Laboratoire de Physique des Matériaux
More informationData Mining: Exploring Data. Lecture Notes for Chapter 3. Introduction to Data Mining
Data Mining: Exploring Data Lecture Notes for Chapter 3 Introduction to Data Mining by Tan, Steinbach, Kumar Tan,Steinbach, Kumar Introduction to Data Mining 8/05/2005 1 What is data exploration? A preliminary
More informationPlastic Bonded Magnets
30 Plastic Bonded Magnets History Development of plastic bonded, injection moulded hard ferrite magnets: End of the 1950s Use: Beginning of the 1960s Development of plastic bonded, injection moulded NdFeB
More informationNUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES
Vol. XX 2012 No. 4 28 34 J. ŠIMIČEK O. HUBOVÁ NUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES Jozef ŠIMIČEK email: jozef.simicek@stuba.sk Research field: Statics and Dynamics Fluids mechanics
More informationEngineering Problem Solving and Excel. EGN 1006 Introduction to Engineering
Engineering Problem Solving and Excel EGN 1006 Introduction to Engineering Mathematical Solution Procedures Commonly Used in Engineering Analysis Data Analysis Techniques (Statistics) Curve Fitting techniques
More informationWhole Numbers and Integers (44 topics, no due date)
Course Name: PreAlgebra into Algebra Summer Hwk Course Code: GHMKUKPMR9 ALEKS Course: PreAlgebra Instructor: Ms. Rhame Course Dates: Begin: 05/30/2015 End: 12/31/2015 Course Content: 302 topics Whole
More informationState of Stress at Point
State of Stress at Point Einstein Notation The basic idea of Einstein notation is that a covector and a vector can form a scalar: This is typically written as an explicit sum: According to this convention,
More informationApplication of Nuclear Magnetic Resonance in Petroleum Exploration
Application of Nuclear Magnetic Resonance in Petroleum Exploration Introduction Darko Tufekcic, consultant email: darkotufekcic@hotmail.com Electromagnetic resonance method (GEOEMR) is emerging as the
More informationEFFECT OF PARTICLE SIZE DISTRIBUTION ON THE MICROSTRUCTURE AND MAGNETIC PROPERTIES OF SINTERED NdFeB MAGNETS
Effect Rev. Adv. of particle Mater. Sci. size 28 distribution (2011) 185189 on the microstructure and magnetic properties of sintered... 185 EFFECT OF PARTICLE SIZE DISTRIBUTION ON THE MICROSTRUCTURE
More informationIron Powder Cores for Switchmode Power Supply Inductors. by: Jim Cox
HOME APPLICATION NOTES Iron Powder Cores for Switchmode Power Supply Inductors by: Jim Cox Purpose: The purpose of this application note is to cover the properties of iron powder as a magnetic core material
More informationDETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES K. Fukushima*, H. Cai**, M. Nakada*** and Y. Miyano*** * Graduate School, Kanazawa Institute of Technology
More informationMagnetic Field Sensors (Hall Generators)
54 Hall Sensors General Information Magnetic Field Sensors (Hall Generators) Hall generator theory A Hall generator is a solid state sensor which provides an output voltage proportional to magnetic flux
More informationPHYS 222 Spring 2012 Final Exam. Closed books, notes, etc. No electronic device except a calculator.
PHYS 222 Spring 2012 Final Exam Closed books, notes, etc. No electronic device except a calculator. NAME: (all questions with equal weight) 1. If the distance between two point charges is tripled, the
More information1051232 Imaging Systems Laboratory II. Laboratory 4: Basic Lens Design in OSLO April 2 & 4, 2002
05232 Imaging Systems Laboratory II Laboratory 4: Basic Lens Design in OSLO April 2 & 4, 2002 Abstract: For designing the optics of an imaging system, one of the main types of tools used today is optical
More informationMATH BOOK OF PROBLEMS SERIES. New from Pearson Custom Publishing!
MATH BOOK OF PROBLEMS SERIES New from Pearson Custom Publishing! The Math Book of Problems Series is a database of math problems for the following courses: Prealgebra Algebra Precalculus Calculus Statistics
More information